is 1141 (1993): seasoning of timber- code of practice is 1141 : 1993 homogenous grain and properties
Post on 06-Jul-2020
Embed Size (px)
Disclosure to Promote the Right To Information
Whereas the Parliament of India has set out to provide a practical regime of right to information for citizens to secure access to information under the control of public authorities, in order to promote transparency and accountability in the working of every public authority, and whereas the attached publication of the Bureau of Indian Standards is of particular interest to the public, particularly disadvantaged communities and those engaged in the pursuit of education and knowledge, the attached public safety standard is made available to promote the timely dissemination of this information in an accurate manner to the public.
“!ान $ एक न' भारत का +नम-ण” Satyanarayan Gangaram Pitroda
“Invent a New India Using Knowledge”
“प0रा1 को छोड न' 5 तरफ” Jawaharlal Nehru
“Step Out From the Old to the New”
“जान1 का अ+धकार, जी1 का अ+धकार” Mazdoor Kisan Shakti Sangathan
“The Right to Information, The Right to Live”
“!ान एक ऐसा खजाना > जो कभी च0राया नहB जा सकता है” Bhartṛhari—Nītiśatakam
“Knowledge is such a treasure which cannot be stolen”
“Invent a New India Using Knowledge”
IS 1141 (1993): Seasoning of timber- Code of practice [CED 9: Timber and Timber Stores]
( pm s;T&m )
SEASONING OF TIMBER - CODE OF PRACTICE
. . ( Second Revision )
@ BIS 1993
BUREAU OF INDIAN STANDARDS MANAK BHAVAN, 9 BAHADUR SHAH ZAFAR MARG
NEW DELHI 110002
Qciober 1993 Prim Grog 10
Timber Sectional Committee, CED 9
This Indian Standard ( Second Revision ) was adopted by the Bureau of Indian Standards, after the draft finalized by the Timber Sectional Committee had been approved by the Civil Engineer- ing Division Council.
Seasoning is the first step in the efficient utilization of timber, especially in this country, where the climatic conditions are very trying for wood work, and where several commercially impor- tant species of wood are hard, heavy and liable to develop defects during drying and in use, unless carefully seasoned. It should be emphasized that all timbers, whether teak or other species, naturally durable or non-durable need proper seasoning in order to give satisfactory service. Seasoning should be regarded as an integral part of timber utilization. With the increased use of several secondary species that possess higher shrinkage than teak, padauk, deodar, rosewood, etc, it has become imperative that adequate attention should be paid to the process of seasoning of wood before use. This has been further necessitated also by the increas- ing availability of short rotation plantation wood of fast growing species under social/agro forestry programmes such as Eucalyptus hybrid, Acacia nilotica, Populus deltoides, Grevillea robusta, etc.
Freshly felled timber contains a large quantity of moisture, in many cases roughly 100 percent based on oven-dry weight of wood, though in some light timbers the quantity of water in green condition is twice as much as the weight of wood substance ( that is, roughly 200 percent ). A well seasoned piece of wood should on the other hand contain about 10 to 12 percent moisture on an average. This would be in equilibrium with the atmospheric humidity in several parts of the country. This degree of seasoning is necessary for proper retention of shape and size of component parts of high class articles, such as cabinet work, railway carriages, panelling, etc. For rough work, and for outdoor uses, drying of timber, -say up to I5 to 25 percent moisture content, is considered enough. This also makes preservative treatment easy and effective.
The process of drying timber, under more or less controlled conditions is called seasoning. During the course of the drying process, timber may develop defects and this is avoided by pro- viding adequate protection against unduly rapid drying condrtions, care in stacking and top weighting of the stacked timber. Timber shrinks during drying; the main objective of seasoning is to eliminate this shrinkage and the associated drying defects before use. Other advantages are, increase in the strength and eIectrica1 resistance of timber, reduction in weight for trans- port purposes, improvement in wood-working qualities including gluing, painting and polishing, and a certain degree of protection from attack by insects and fungi depending upon the moisture content to which timber has been seasoned. Seasoned timber should be stored under cover protected from rain and other forms of precipitation.
Sawn timber for special purposes may be given an antishrink treatment and a recommended method is given in Annex A.
This standard was first published as tentative standard in 1958 and then revised in 1973. Apart from conventional seasoning processes, namely air and kiln seasoning, this second revision also details certain special seasoning processes and preseasoning treatments that may be adopted to reduce drying times, costs and defects, conserve energy or avoid pollution. This revision also incorporates guidelines on the technique of sawing of logs of certain species containing severe growth stresses to minimize warping on the saw and to minimize surface cracking during subse- quent seasoning of the sawn timber.
The composition of the technical committee responsible for formu!ation of this standard is given in Annex E.
For the purpose of deciding whether a particular requirement of this standard is complied with, the final value, observed or calculated, expressing the result of a test or analysis, shall be rounded off in accordance with IS 2 : 1960 ‘Rules for rounding off numerical values ( revised )‘. The number of significant places retained in the rounded off value should be the same as that of the specified value in this standard.
IS 1141 : 1993
SEASONING OF TIMBER-CODE OF PRACTICE
( Second Revision )
This standard covers CIassification of timbers for seasoning purposes; preliminary treatment and storage; stacking practice; pre- seasoning treatment; seasoning methods; kiln schedules for seasoning different species of timbers; pre and post-treatment seasoning; kiln operation procedure; measures for control of warp; and inspection, transport and storage of seasoned timber. General guidelines are also included for seasoning of bamboo.
NOTE - The design and construction of seasonmg kilns, recommended moisture contents for seasoned timber and methods of determination of moisture content are covered in separate Indian Standards, namely, IS 7315 : 1974, IS 287 : 1993 and 1s 11215 : 1991 respectively.
The following Indian Standards are necessary adjuncts to this standard:
287 : 1993
401 : 1982
707 : 1976
6313 ( Part 2 ) : 1981
7315 : 1974
11215 : 1991
Recommendations for maxi- mum permissible moisture content of timber used for different purposes ( third revision ) Code of practice for preserva- tion of timber ( third revision)
Glossary of terms applicable to timber technology and utilization ( second revision ) Code of practice for anti- termite measures in buildings: Part 2 Pre-constructional chemical treatment measures (first revision )
Guidelines for design, installa- tion and testing of timber seasoning kilns Methods for determination of moisture content of timber and timber products
3 TERMINOLOGY For the purpose of this standard the definitions given in IS 707 : 1976 shall apply.
4 CLASSIFICATION OF TIMBERS FOR SEASONING PZJRPOSES
4.1 For the purpose of seasoning, timbers shall be classified into the following three classes depending upon their behaviour with respect to cracking and splitting, and drying rate:
a) Class A : Highly refractory b) Class B : Moderately refractory, and
c) Class C : Non-refractory
4.2 Highly Refractory Woods
These are slow drying and difficult to season free from cracking and splitting. Examples are heavy structural timbers, such as sal ( Shorea robusta ) and laurel ( TerminaIia alata ).
4.3 Moderately Refractory Woods
These may be seasoned free from surface and end cracking within reasonable short periods, given a little protection against rapid drying conditions. Examples are moderately heavy furniture class of timbers, such as sissoo ( Dalbergia sissoo ) and teak ( Tectona grandis ).
4.4 Non-refractory Woods
These may be rapidly seasoned free from surface and end cracking even in the open air and sun. If not rapidly dried, they develop blue stain and mould on the surface. Examples are light broad leaved ( hardwood) species for packing cases, such as semul ( Bombax spp. ) and salai ( Boswellia serratu ), and all coniferous species.
4.5 Classification of commercially important Indian timbers into the above three classes is given in Annex B.
5 DEFECTS FOR SEASONING PURPOSES
5.1 For seasoning purposes, defects in timber shall be grouped as follows:
a) Drying defects, and
b) Defects not associated with drying.
5.2 Drying defects develop in timber as a result of drastic drying conditio